Spatial distribution of phases during gradual magnetostructural transitions in copper(ii)-nitroxide based molecular magnets.
Fedin, Matvey V.; Veber, Sergey L.; Bagryanskaya, Elena G.; Romanenko, Galina V.; Ovcharenko, Victor I.; Dalton transactions (Cambridge, England : 2003) 44 (2015) 18823–18830; doi:10.1039/c5dt03441h

data_7036693
_publ_section_title
;
 Spatial distribution of phases during gradual magnetostructural
 transitions in copper(ii)-nitroxide based molecular magnets.
;
_journal_issue                   43
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              18823
_journal_page_last               18830
_journal_paper_doi               10.1039/c5dt03441h
_journal_volume                  44
_journal_year                    2015
_chemical_formula_sum            'C23 H23 Cu F12 N4 O6'
_chemical_formula_weight         742.99
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/6
_audit_update_record
;
2015-08-12 deposited with the CCDC.
2015-09-29 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 125.6211(17)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   30.6714(18)
_cell_length_b                   9.5911(5)
_cell_length_c                   25.970(2)
_cell_measurement_reflns_used    9848
_cell_measurement_temperature    240(2)
_cell_measurement_theta_max      67.53
_cell_measurement_theta_min      3.58
_cell_volume                     6210.2(7)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_diffrn_ambient_temperature      240(2)
_diffrn_measured_fraction_theta_full 0.989
_diffrn_measured_fraction_theta_max 0.986
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0287
_diffrn_reflns_av_unetI/netI     0.0190
_diffrn_reflns_laue_measured_fraction_full 0.989
_diffrn_reflns_laue_measured_fraction_max 0.986
_diffrn_reflns_limit_h_max       36
_diffrn_reflns_limit_h_min       -33
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       30
_diffrn_reflns_limit_l_min       -30
_diffrn_reflns_number            36166
_diffrn_reflns_point_group_measured_fraction_full 0.989
_diffrn_reflns_point_group_measured_fraction_max 0.986
_diffrn_reflns_theta_full        67.679
_diffrn_reflns_theta_max         67.811
_diffrn_reflns_theta_min         3.545
_exptl_absorpt_coefficient_mu    2.067
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            dark
_exptl_crystal_density_diffrn    1.589
_exptl_crystal_description       bulk
_exptl_crystal_F_000             2992
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.18
_refine_diff_density_max         0.434
_refine_diff_density_min         -0.351
_refine_diff_density_rms         0.041
_refine_ls_extinction_coef       0.00008(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.021
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     554
_refine_ls_number_reflns         5563
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.021
_refine_ls_R_factor_all          0.0393
_refine_ls_R_factor_gt           0.0380
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0678P)^2^+4.4323P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1119
_refine_ls_wR_factor_ref         0.1134
_reflns_Friedel_coverage         0.000
_reflns_number_gt                5269
_reflns_number_total             5563
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c5dt03441h2.cif
_cod_data_source_block           240
_cod_depositor_comments
'Adding full bibliography for 7036688--7036694.cif.'
_cod_original_cell_volume        6210.1(7)
_cod_database_code               7036693
_shelxl_version_number           2014/6
_shelx_res_checksum              28597